Improving poly(arylene piperidinium) anion exchange membranes by monomer design

Energy conversion devices such as alkaline fuel cells and water electrolyzers rely critically on durable anion exchange membranes (AEMs) with high hydroxide conductivity. In this context, poly(arylene piperidinium)s derived from...


Introduction
A broad world-wide implementation of fuel cell powered vehicles and devices calls for the development of a more sustainable and cost-effective alternative to the proton exchange membrane fuel cell (PEMFC).][10][11][12][13] AEMs should possess high ion conductivity at a limited ionic content to avoid excessive water uptake and swelling that will compromise the mechanical strength.The long-term structural integrity and properties of the AEMs are however greatly challenged by the severe alkaline operating conditions in these devices.Both the polymer backbone and the tethered cations are prone to degrade via hydroxide attack, resulting in loss of mechanical integrity and ion conductivity, respectively. 141][22] In addition, the alkaline stability of various organic cations, including imidazolium, 23 quaternary ammonium (QA) [24][25][26][27] and organometallic cations, 28,29 have been studied as model compounds to identify suitable candidates. 30In this context, different N-heterocyclic QA cations have emerged as synthetically accessible and generally highly alkali-stable ion-exchange groups.][36] Poly(arylene piperidinium)s (PAPs) have piperidinium rings directly attached to the backbone structure and constitute a rather new class of polymers which has drawn increasing attention as membrane materials, primarily because of their stiff aromatic backbone, high alkaline stability, tunable structure, and relative ease of synthesis and processing (Scheme 1).Commercially available 4-piperidone and N-methyl-4piperidone monomers and different arenes enable straightforward synthesis of high-molecular weight PAPs by superacid-mediated polyhydroxyalkylations, followed by a suitable quaternization to introduce the desired piperidinium-type cation.In general, AEMs based on PAPs with moderate ion exchange capacities (IECs) show a well-controlled water uptake, high hydroxide ion conductivity and chemical stability.For example, an AEM based on poly(p-terphenyl dimethylpiperidinium) displayed no structural change aer storage in 2 M aq.NaOH at 60 C for 15 days. 37Subsequently, the ex-situ stability of PAP-based AEMs has been veried to exceed 1500 h in 1 M aq.NaOH at 80 C. 38,39 A number of different successful approaches have been reported to further improve membrane durability and performance, including the introduction of exible spacers, 40 arrangements with multiple cations, 41,42 crosslinking, [43][44][45] branching 46 and reinforcement. 47For example, we recently reported on a series of cationically modied poly(biphenyl piperidine)s which retained >92% of the cations aer storage in 2 M aq.NaOH at 90 C for 30 days. 48This was achieved by leaving the piperidine groups in the backbone nonquaternized and hence far less sensible to hydroxide attack and degradation.
Although quite alkali-stable, PAP-based AEMs are still susceptible to ionic loss via, e.g., ring-opening Hofmann elimination and substitution in harsh alkaline environments.A high ionic loss relative to model piperidinium cations has been partly attributed to the conformational distortion of the piperidinium ring directly attached to the rigid PAP backbone. 37urthermore, the ionic loss has been observed to accelerate when the possibilities for ring relaxation was further restricted by the spirocyclic arrangement of the ASU cation. 49Hence, the alkaline stability of these cations is highly dependent on precisely how they are attached to the polymer backbone, 9,50 and in many cases on the rigidity of the backbone itself. 17,51roviding a high local mobility of the cations by tethering via exible spacers has shown to increase their resistance against hydroxide attack.In order to reduce ionic loss by b-elimination at the spacer chain, it is advantageous to attach the piperidinium rings via the 4-position instead of the 1(N)-position.In this way, all the b-hydrogens are placed in the better protected ring structure, which produces substantially more stable AEMs. 52ith the aim to further enhance membrane properties and stability beyond that of AEMs based on PAP, we have in the present work designed and synthesized a new piperidinefunctional triuoromethylketone monomer, and then prepared and studied a series of poly(arylene alkylene piperidinium)s (PAAPs) tethered with DMP and ASU cations (Scheme 1).The monomer was designed to place the cations pendent to the polymer backbone in order to lessen the conformational distortion of the rings by the stiff backbone and increase the ring strain relaxation.The PAAPs were prepared in superacidmediated polycondensations with different arene monomers, followed by quaternization reactions to produce the cations.Solution-cast AEMs were characterized with regard to water uptake, hydroxide conductivity, morphology, thermal and alkaline stability.A special emphasis was placed on alkaline stability and ion-loss mechanisms, and the results were benchmarked against PAP reference AEMs.

Monomer synthesis and characterization
Piperidone and various triuoromethyl ketones have been widely employed in Friedel-Cras type polycondensations with electron-rich aromatic compounds to prepare linear, highmolecular-weight polymers functionalized with different cationic groups (Scheme 1). 20,37In the present work, the monomer 2,2,2-triuoro-1-(4-piperidine)ethanone (TFPip) was designed to improve the alkaline stability of AEMs, and was subsequently synthesized as a hydrochloride salt in two steps, starting from commercially available 4-piperidinecarboxylic acid (Fig. 1).In the rst step, the carboxylic moiety was converted to a triuoroacetyl group by a reaction with triuoroacetic anhydride (TFAA), in the presence of pyridine, followed by hydrolysis/decarboxylation in water.In parallel, the piperidine N-H functionality underwent N-triuoroacetylation.The majority of the piperidine groups remained in the protected form aer the hydrolysis, and a mixture of the intermediate and the nal TFPip product (salt-free) was detected in the crude product (Fig. S1 †).Still, this did not interfere with the subsequent synthesis and purication.In the second step, a complete deprotection of the mixed intermediate product was carried out in concentrated HCl at 100 C overnight.Finally, the pure TFPip hydrochloride salt was obtained aer recrystallization in acetonitrile.The synthesis was based on 26 g 4- piperidinecarboxylic acid which was divided in two separate reactions conducted in parallel before combining the batches in the second step.
The successful synthesis and purication of TFPip was conrmed by 1 H NMR spectroscopy (Fig. 1).The a (c) and b (b) protons of the piperidine ring were observed as split signals located between 2.8-3.3 ppm and 1.6-1.9ppm, respectively.The methine proton (a) emerged at around 1.9 ppm and was partly overlapped with one of the b (b) proton signals.A broad singlet at 8.9 ppm was assigned to the protonated secondary piperidine ring (d).The molar mass of TFPip was also conrmed by highresolution mass spectroscopy (Table S1 †).

Synthesis and characterization of poly(arylene alkylene piperidinium)s
Superacid-mediated polyhydroxyalkylations involving TFPip and different electron-rich arene monomers were carried out as shown in Scheme 2. The electron-withdrawing triuoromethyl substituent gave the TFPip monomer sufficient electrophilicity to react with common arenes in the superacid medium. 54uring the polycondensations, the ketone moiety of TFPip is protonated to generate a dication to react with the arene monomer.In general, TFPip showed moderate reactivity, as evidenced by the long polymerization periods required to reach high molecular weights.Consequently, we used a high molar excess of TFPip (up to 40%) in order to accelerate the polymerization rate.The polycondensations were carried out in dichloromethane (DCM) at 20 C and the resulting polymers containing p-terphenyl (pT), m-terphenyl (mT), biphenyl (B) and 9,9-dimethyl-9H-uorene (dF) units were denoted PpTPip, PmTPip, PBPip and PdFPip, respectively.Their structures were subsequently veried by 1 H NMR spectroscopy (Fig. 2 and S2 †) aer addition of triuoroacetic acid (TFA) to the DMSO-d 6solutions.The signals located between 1.5 and 3.9 ppm corresponded to piperidine ring protons (a)-(c) and were found in all the polymer spectra.Moreover, the signal of the protonated secondary N + -H 2 groups (d) appeared between 8.0 and 8.5 ppm as distinctly split singlets.In polyhydroxyalkylations involving piperidone, signals originating from vinylic groups formed in elimination reactions are frequently observed at 6.2 and 4.0 ppm. 37These side reactions limit the molecular weight, and thus the AEM properties.In the present case, no traces of elimination products were detected in any of the polycondensation experiments, which shows that the TFPip monomer is less sensitive to elimination than piperidone during polyhydroxyalkylations.In the protonated form, the polymers were readily soluble in common organic solvents, such as dimethyl sulfoxide (DMSO), N-methyl-2-pyrrolidone (NMP) and acetone, but were non-soluble in DCM, chloroform and tetrahydrofuran (THF).Scheme 2 Synthesis and designations of the cationic polymers prepared via superacid-mediated polyhydroxyalkylations and quaternizations.
PAAPs were prepared by quaternizations of the precursor polymers (PpTPip, PmTPip, PBPip and PdFPip) using methyl iodide and 1,5-dibromopentane, respectively, which resulted in the formation of DMP and ASU cations, respectively.Because of the limited solubility in solvents commonly used in size exclusion chromatography (e.g., chloroform and THF), as well as a lack of suitable reference samples, the molecular weight of the polymers carrying the DMP cation was estimated by intrinsic viscosity ([h]) measurements in 0.1 M LiBr in DMSO at 25 C.The results (Table 1) showed that high molecular weights were achieved in polycondensations involving the terphenyls (pT and mT), which was further supported by the good lm-forming properties of these samples.However, it was not possible to reliably measure the intrinsic viscosities of PBDMP and PdFDMP, suggesting low molecular weights when the polymerizations involved biphenyl and dimethyluorene, respectively.This may be attributed to the comparatively low reactivity of the latter arenes in the polycondensations.Although freestanding membranes were cast from DMSO solutions of PBDMP and PBASU, they were rather brittle in the dry state, and extremely so when hydrated and thus difficult to handle.This was most probably a consequence of the high IEC, the rather high backbone exibility, combined with limited molecular weights.Therefore, cationic polymers based on pT and mT were excellent candidates for use as AEMs, whereas those based on biphenyl and dimethyluorene may be suitable as high-IEC ionomers in the electrode layers.Because of the high reactivity of pT, we chose to further optimize this polycondensation.The results showed values of [h] between 0.52 and 1.37 dL g À1 depending on the reaction conditions.Details of the different polymerizations and the products are described and summarized in the experimental section (Table 2).The PpTPip sample reaching the highest intrinsic viscosity (Table 2, entry 4) was used in the preparation of the AEMs further described below.

Membrane preparation and morphology
Transparent membranes with excellent robustness and exibility were prepared from PpTDMP, PpTASU, PmTDMP and PmTASU solutions in NMP at 80 C. The AEMs were ion-exchanged to the Br À form and subsequently stored in deionized water prior to characterization.The ion exchange capacity (IEC) was determined by Mohr titrations.As shown in Table 1, the results were in excellent accordance with the theoretical values expected from the polymer structures, which indicated the completeness of the quaternizations.The morphology of the AEMs was studied by small-angle X-ray scattering (SAXS) and the results are shown in Fig. 3.As indicated by the arrows, ionomer peaks indicated by scattering maxima were observed for PpTDMP and PpTASU.Specically, the ionomer peak of PpTDMP were found at q ¼ 1.6 nm À1 , which corresponded to a characteristic separation distance (d) of 3.9 nm.PpTASU displayed a similar scattering prole with the ionomer peak at q ¼ 1.3 nm À1 and a corresponding d-spacing of 4.8 nm.In addition, a second scattering maximum was observed for these two AEMs at q ¼ 5.6 nm À1 .This corresponded to d ¼ 1.1 nm, which approximately equals the length of a terphenylene unit.In comparison, benchmark poly(p-terphenyl piperidinium) (PTPipQ100) and poly(biphenyl piperidinium) (PBPipQ100), both derived from piperidone (Scheme 1), displayed single ionomer peaks at q ¼ 1.6 and 2.5 nm À1 , respectively, and showed no scattering maxima around q ¼ 5.6 nm À1 .Furthermore, AEMs based on mT showed a distinctly different SAXS prole than their pT counterparts.A broad ionomer peak centered around q ¼ 3.1 nm À1 was detected for PmTDMP.This can be explained by the higher exibility of the m-terphenylene conformation which potentially facilitated ionic aggregation.PBDMP and PBASU exhibited an ionomer peak around 2.3 and 2.2 nm À1 , respectively, indicating their distinct phase-separated morphology.

Thermal stability
The thermal stability of the precursor polymers and the AEM samples were studied by thermogravimetrical analysis (TGA) (Fig. 4) by recording the thermal decomposition temperature at 95% weight loss (T d,95 ) (Table 1).The precursor polymers PmTPip and PpTPip both degraded in single steps at T d,95 ¼ 376 and 385 C, respectively, attributed to their stiff and aromatic backbone structures.Aer the quaternizations, the AEMs surprisingly reached an even higher thermal stability.The PmTDMP and PpTDMP samples displayed signicantly higher T d,95 values at 428 and 452 C, respectively, while PpTASU and PmTASU had lower values, i.e., T d,95 ¼ 389 and 394 C, respectively.As frequently reported, QA functionalized AEMs normally decompose at lower temperatures than the non-functionalized precursors.For example, the T d,95 values of poly(arylene piperidinium) s 37,43 and poly(arylene alkylene)s 20,55 have previously been reported to be lower than their corresponding precursors polymers.In the present study, the opposite trend can be attributed to the nature of the precursor polymers, where the piperidine groups remained protonated and carried TFSA À counter ions.We speculated that the presence of the triate ions weakened the piperidine unit and therefore impaired its thermal stability.The thermal stability of samples based on the two different backbone congurations, i.e.,   pT and mT, showed little difference.TGA traces of samples containing biphenyl and dimethyluorene units indicated a similar degradation behavior as those based on pT and mT (Fig. S3 †).

Water uptake and swelling ratio
The presence of water is crucial for the function of an AEM.An ideal uptake of water facilitates efficient ion transport in the membrane, while an excessive water uptake leads to swelling and loss of mechanical robustness and even to disintegration.The water uptake and swelling behavior of the present AEMs in the OH À form were gravimetrically determined (Fig. 5a-d and Table 1).As expected, the water uptake of the AEMs increased with temperature and IEC.The PBDMP and PBASU membranes had a high water uptake because of their high IECs and backbone exibility.The fully hydrated samples were difficult to handle and hence the water uptake and swelling were not measured.When the m-terphenyl backbone was employed, the water uptake was considerably more restricted.For example, PmTASU showed a water uptake of 105 and 341% at 20 and 80 C, respectively.At a higher IEC, the water uptake of PmTDMP reached 144% and over 400% at 20 and 80 C, respectively.Notably, the AEM samples, although so, remained intact with such high water contents.As expected, when the stiffer p-terphenyl was employed, the water uptake of the AEMs became even more constrained.PpTDMP showed a water uptake between 78 and 104% between 20 and 80 C. With the bulkier ASU cation and slightly lower IEC, PpTASU demonstrated a lower water uptake, i.e., 43-81% in the same temperature range.These AEMs also displayed moderate inand through-plane swelling, around 20% even at 80 C. The restricted water uptake of the PpT AEMs may primarily be explained by the higher rigidity of the p-terphenylene backbone compared with the m-terphenylene counterpart.However, the higher molecular weight of the former, as indicated by the [h] values, also limited the water uptake and swelling by improving the viscoelastic properties.This relationship was corroborated by data obtained with AEMs prepared from PpTDMP samples with different [h] values, which showed that the water uptake decreased from 174 to 104% at 80 C as [h] increased from 0.52 to 1.37 dL g À1 (Fig. 5b).The large dependence on the molecular weight emphasized the necessity to optimize the polymerization to obtain high-performance AEMs.

Ion conductivity
High OH À conductivity is a key property for AEMs which is dependent on several factors, including the IEC, water uptake, morphology and temperature.In the present study, the OH À conductivity of PAAP AEMs in the fully hydrated (immersed) state was measured by electrochemical impedance spectroscopy (EIS) between 20 and 80 C. As shown in Fig. 6a-c, the conductivities of the PAAP AEMs increased with temperature and water uptake as anticipated.Overall, high conductivities were reached for all the AEMs (Table 1) and an Arrhenius behavior was shown (Fig. 6a and b).The most conductive PAAP AEM was PpTDMP, reaching a OH À conductivity of 79 and 178 mS cm À1 at 20 and 80 C, respectively.Similarly, PmTDMP had OH À conductivities of 78-169 mS cm À1 at the same IEC.Furthermore, AEMs carrying the bulky ASU cations (PpTASU and PmTASU) also displayed high conductivities, between 67 and 157 mS cm À1 , despite the lower IEC.The relationship between the OH À conductivity and the hydration number (l) of the AEMs is given in Fig. 6c.When AEMs with different backbone structures were compared, it was obvious that PpT AEMs were more effective ion conductors than the PmT AEMs, as seen by the much steeper conductivity increase with l compared to the latter AEMs.A dilution effect by which excessive water uptake decreased the charge carrier concentration, resulting in less efficient ion transport, was clearly observed for the PmT AEMs.The OH À conductivity of PpTDMP was compared with benchmark PAP AEMs.Here, the homopolymer PTPipQ100 (ref.56) was selected because it has the same terphenyl backbone and piperidinium cation (Scheme 3) as PpTDMP.The copolymer PTPipQ83 was included because of a similar IEC and water uptake in comparison with PpTDMP.As shown in Fig. 6a, PpTDMP reached higher conductivity values than the two benchmarks based on PAP.This could be attributed to the combination of the high molecular weight, reasonably high IEC, and the cationic arrangement of PpTDMP, which led to a more distinct phase separation of the AEM (Fig. 3).Moreover, the conductivity of PTPipQ100 increased only slowly with increasing water content (l), most probably due to the high IEC and overall water uptake, leading to a dilution effect (Fig. 6c).

Alkaline stability
One critical factor that hampers the development of durable AEMFCs is the lack of sufficient long-time chemical stability of currently available AEMs under alkaline environment.The rational design of monomer TFPip was expected to provide polymers with a cationic arrangement which enhances the resistance against OH À attack, especially in relation to PAP AEMs based on piperidone (Scheme 1).In order to investigate this, the two benchmark AEMs based on PAPs prepared from piperidone, PTPipQ83 and PTPipQ100, were included in the alkaline stability study (Scheme 3).The copolymer PTPipQ83 had a similar water uptake as PpTDMP, which presumably gave a comparable effect of the hydration level on the stability. 57ere, the alkaline stability and degradation were investigated by 1 H NMR spectroscopy in order to probe the active degradation mechanisms and assess the ex situ lifetime of the AEMs.Samples were rst immersed in alkaline media, initially 2 M aq.NaOH at 90 C during 20-100 days.Subsequently, the AEM samples were also studied aer storage in 5 M aq.NaOH at the same temperature for 10 and 20 days.All the samples retained their mechanical integrity and robustness aer these severe testing conditions. 1 H NMR spectra of the AEM polymers before and aer storage in alkali were recorded aer dissolution in DMSO-d 6 with addition of TFA (Fig. 7, 8 and S4-S10 †).
The degradation mechanisms of the DMP and ASU cations have already been widely studied and reported. 37,48,49Typically, in a severe alkaline environment, both cations undergo Hofmann elimination at b-hydrogens, or ring-opening nucleophilic substitution at a-carbons.Methyl substitution occurs exclusively for the DMP cations.9][60] For instance, Hofmann elimination is depressed for the DMP cation due to the high energy transition state, which instead cause degradation via methyl substitution to dominate.This may in turn be circumvented by replacing the methyl groups with a second 6-membered ring to form a spiro cation, i.e., the ASU cation.This cation successfully demonstrated a longer half-life (110 h for ASU versus 87.3 h for DMP at 160 C in 6 M aq.NaOH). 24However, the reverse situation has oen been observed when these N-alicyclic cations are incorporated into various polymer structures, such as PAPs. 50,52ofmann elimination is dominant in most cases, 37 which has been attributed to a distortion of the ring conformation imposed by the rigid arylene backbone.In fact, ionic loss through elimination has been found to increase with the rigidity of the backbones. 51In AEMs the ASU cation has been found to be more prone to degrade compared with the DMP cation, which is in contrast to the results on the corresponding model compounds.
In the present study, structural changes of the AEM samples were detected by 1 H NMR spectroscopy aer storage in 2 M aq.NaOH at 90 C for 20 days, even though the new signals from the degradation products were very small, and the ionic loss was only quantiable aer 60 day's storage (Fig. S5-S8, d-g †).Consequently, the AEMs were treated under harsher conditions to accelerate the ionic loss, and 1 H NMR spectra were recorded aer immersion in 5 M aq.NaOH at 90 C for 10 and 20 days.Fig. 7 shows the spectra of PpTDMP and PpTASU before and aer the aforementioned treatment, and the spectra of the other AEM samples are provided in Fig. S7-S10.† As shown in Fig. 7c, the signals at 5.1 (c 1 ) and 5.4 (b 1 ) ppm were ascribed to the vinyl groups of the Hofmann elimination products, along with the tertiary proton signal at 9.48 ppm (d 1 ).As expected, the three signals had intensity ratios of 2 : 1 : 1. Traces of methyl and ring-opening substitution were also detected, as indicated by two small additional signals (d 2 and d 3 ) from protonated tertiary piperidine between 9.0 and 9.5 ppm.When it comes to PpTASU, another set of vinylic signals was detected (Fig. 7f), suggesting Hofmann elimination in both ASU rings (inner and outer).In addition, the alkaline stability of PpTDMP was compared with the benchmark PAP AEMs, as shown in Fig. 8. Aer alkaline storage, the PAP reference materials showed distinct signals from vinylic protons between 4.8 and 6.8 ppm, originating from Hofmann elimination. 37Lastly, the 1 H NMR spectra of PmTDMP and PmTASU, presented in Fig. S7 and S8, † showed that AEMs based on PmT degraded in a similar manner as the PpT-based AEMs, despite the different backbone congurations.
The ionic loss of the AEMs was calculated by comparing the integral of the (protonated) amine signals around 9 ppm, originating from the degradation of piperidinium, with the intensity of all the aromatic signals (7-8 ppm), which remained unaffected by the alkaline treatment.The results are summarized in Table 3 and revealed that PpTDMP was the most stable AEM in the present study, with a mere 14% ionic loss, aer storage in 5 M NaOH at 90 C for 20 days.Under the same conditions, the reference samples PTPipQ83 and PTPipQ100 showed an ionic loss of 52 and 42%, respectively, which was signicantly higher than that of PpTDMP.Moreover, in PpTDMP half of the degradation occurred via Hofmann elimination, accounting for 7% ionic loss.In comparison, Hofmann elimination was the primary pathway in the benchmark AEM, corresponding to 42% ionic loss for PTPipQ83 (out of a total 52% ionic loss).The most possible reason for the superior alkaline stability of the present AEMs lies in the more favorable cationic arrangement.First of all, the piperidinium rings are attached in the 4-position.This greatly enhances the alkaline stability of the cation, 52 in comparison to corresponding piperidinium rings tethered at the 1(N)-position. 55Furthermore, the ring strain imposed by the rigid polymer chain are alleviated in, e.g., PpTDMP, as opposed to the benchmark PTPipQ100 where the cations are directly incorporated in the backbone.In PpTDMP, the piperidinium rings are separated from the backbone, which signicantly facilitates the ring relaxation to impede ionic loss.This was supported by the reduced ionic loss via Hofmann elimination, in comparison to the PAP benchmark materials.Electron-withdrawing substituents located in the vicinity of cations usually decrease their alkaline stability. 59owever, in the present case the quite strongly electronwithdrawing triuoromethyl group seemed to be distant enough from the piperidinium ring in the polymer structure not to deteriorate its alkaline stability.

Polymer synthesis
Synthesis of monomer TFPip.The ketone monomer 2,2,2-triuoro-1-(4-piperidine)ethanone (TFPip) in the hydrochloric salt form was synthesized in two steps as presented in Fig. 1.Isonipecotic acid (13 g, 100 mmol, 1 equiv.)was dissolved in toluene (40 mL) in a 250 mL three-neck round bottom ask, and TFAA (78 mL, 561 mmol, 5.58 equiv.) was slowly added while stirring.The reaction mixture was cooled to 0 C using an ice bath.Next, pyridine (65 mL, 807 mmol, 8.02 equiv.) was added dropwise.Aer the addition was completed, the temperature was increased to 50 C, and the reaction was allowed to proceed for 48 h under nitrogen atmosphere.The reaction solution was then cooled to 0 C, and deionized water (143 mL) was added dropwise before raising the temperature to 45 C for 2 h.Aer the solution separated into layers, it was extracted with ethyl acetate (EtOAc, 4 Â 125 mL).The organic phase was washed with deionized water (200 mL), saturated Na 2 CO 3 (200 mL), and a saturated NaCl (200 mL) solution, before drying with Na 2 SO 4 .Following removal of the solvent using a rotary evaporator, the pure product was separated by dry column vacuum chromatography (DCVC) using EtOAc : heptane (0 : 100 to 55 : 45) as eluent.The still impure product was added to a 100 mL round bottom ask lled with concentrated HCl (50 mL) and deionized water (150 mL) and heated to 100 C and le stirring overnight.The solution was cooled to room temperature, and the solvent was evaporated to obtain a dark solid, which was recrystallized from acetonitrile to gain the nal product as a light tan crystal.This gave 25.2 g product at a total isolated yield of 58%.
Synthesis of precursor polymers PpTPip, PmTPip, PBPip and PdFPip.Polymerizations were performed according to the example that follows.In a 50 mL round bottom ask, p-terphenyl (3.0 g, 13.0 mmol, 1 equiv.)and TFPip (3.4 g, 15.6 mmol, 1.2 equiv.)were added with DCM (7 mL).The mixture was cooled to 0 C with an ice bath before dropwise adding TFSA (14 mL, 158.2 mmol, 12.2 equiv.).When the highly viscous reaction mixture impeded the stirring aer ca. 12 days, the reaction was quenched by rst diluting the mixture with NMP and then precipitating the product into iced water.The white ber-like precipitate was ltered and washed several times with deionized water, and nally dried under vacuum at room temperature for 24 h.
Quaternization.The cationic polymers PpTDMP, PmTDMP, PBDMP, and PdFDMP were prepared through quaternization reactions using methyl iodide (MeI) as methylation agent and K 2 CO 3 as base in NMP or DMSO.The synthesis of PpTDMP is described here as an example.PpTPip (0.6 g, 1.1 mmol, 1 equiv.),K 2 CO 3 (0.455 g, 3.3 mmol, 3 equiv.),and MeI (0.34 mL, 5.5 mmol, 5 equiv.)were mixed with 10 mL NMP in a 25 mL round bottom ask and stirred at room temperature for 48 h.During the reaction process, the ask was covered with foil to prevent light-induced degradation of MeI.The product carrying DMP cations was precipitated in an IPA/diethyl ether mixture and repeatedly washed with IPA and water, before ltered off and dried under vacuum to yield PpTDMP as a light yellow powder.
The precursor polymers were also functionalized with pendant N-spirocyclic cations via cyclo-quaternization using 1,5-dibromopentane in the presence of DIPEA as the base.Here, the preparation of PpTASU will serve as an example.A solution of PpTPip (0.6 g, 1.1 mmol, 1 equiv.) in NMP (10 mL) was heated to 80 C.Meanwhile, a solution of 1,5-dibromopentane (0.164 mL, 1.2 mmol, 1.1 equiv.)and DIPEA (1.04 mL, 5.52 mmol, 5 equiv.) in NMP (14 mL) was vigorously stirred in a 50 mL round bottom ask at 80 C. Subsequently, the polymer solution was added slowly dropwise to the reagent ask.The reaction solution was stirred at 80 C for 48 h.Next, the homogeneous darkred solution was cooled to room temperature and the product was precipitated in a diethyl ether/IPA mixture, further washed with fresh diethyl ether, 1 M aq.NaBr and then with deionized water.Finally, the product was dried under vacuum at room temperature to give an orange product.
Description of membrane preparation and characterization methods can be found as ESI.†

Conclusions
A series of PAAPs were prepared and studied with the aim to further enhance the alkaline stability of N-alicyclic QA cations attached to rigid polymer backbones.To that end, the TFPip monomer was rst designed with a reactive triuoromethyl ketone group and a piperidine functionality, and then synthesized using a straightforward procedure.PAAPs based on TFPip were successfully prepared in superacid-mediated polycondensations and subsequent quaternizations to obtain DMP and ASU cations, respectively.Polymers based on biphenyl and dimethyluorene took up too much water, and may instead be suitable ionomers for catalyst layers.In contrast, the corresponding p-and m-terphenyl polymers formed AEMs with excellent mechanical robustness and high OH À conductivity.Optimization of the polymerization conditions was important in order to reach high molecular weights, which resulted in suppressed water uptake and swelling of the corresponding AEMs without compromising their high OH À conductivity.Moreover, beneting from the cationic arrangement, poly(terphenyl alkylene piperidinium)s showed signicantly enhanced the alkaline stability compared to corresponding benchmark poly(terphenyl piperidinium)s prepared from piperidone where the cyclic cations are directly connected to the rigid polymer backbone.Incorporating the cations into the polymer structure in such a way that the backbone and the cyclic cation do not share any atoms, as in the present case, most probably signicantly facilitated the ring relaxation which impeded ionic loss.This work provides valuable insights into the molecular design of high performance alkali-stable AEMs.Future work will focus on evaluations of the new PAAP materials in AEMFC and AEMWE.

Fig. 1
Fig. 1 Synthetic route to monomer TFPip and 1 H NMR spectrum of an isolated sample in the hydrochloride salt form, recorded in DMSO-d 6 .

Fig. 3
Fig. 3 SAXS profiles of the PAAP AEMs.For comparison, scattering data of PTPipQ100 and PBPipQ100 are also shown.

Fig. 4 Fig. 5
Fig. 4 TGA traces of the protonated precursor polymers in the TFSA À form and the AEMs in the Br À form recorded under N 2 atmosphere at a heating rate of 10 C min À1 : samples based on (a) pT and (b) mT, respectively.

Fig. 6
Fig. 6 OH À conductivity of the AEMs in the fully hydrated (immersed) state as a function of (a) and (b) T À1 and (c) the hydration number (l).

Scheme 3
Scheme 3 Molecular structures of a representative PAAP, PpTDMP prepared from TFPip (a), and two corresponding benchmark PAPs for reference: PTPipQ100 (b) and PTPipQ83 (c), both derived from piperidone (counter ions omitted).

Fig. 8 1 H
Fig. 8 1 H NMR spectra of (a) and (b) PpTDMP and the benchmark AEMs (c) and (d) PTPipQ100 and (e) and (f) PTPipQ83 before and after storage in 5 M aq.NaOH at 90 C for 20 days.

Table 1
Properties of the AEMs a Calculated from the polymer structures in the Br À form (OH À form within parentheses).b Measured in the OH À form.c Measured in DMSO at 25 C.

Table 2
Polymerization conditions of PpTPip and the properties of the corresponding PpTDMP AEMs a Measured in DMSO at 25 C. b Measured in the OH À form.

Table 3
Ionic loss of the AEMs obtained by 1 H NMR analysis after storage in 5 M aq.NaOH at 90 C for 20 days